LAMINATED COMPOSITE PLATES

 Dorthy Gwendoline Carpenter
 8 months ago
 Views:
Transcription
1 LAMINATED COMPOSITE PLATES David Roylance Department of Materials Science and Engineering Massachusetts Institute of Technology Cambridge, MA February 10, 2000 Introduction This document is intended to outline the mechanics of fiberreinforced laminated plates, leading to a computational scheme that relates the inplane strain and curvature of a laminate to the tractions and bending moments imposed on it. Although this is a small part of the overall field of fiberreinforced composites, or even of laminate theory, it is an important technique that should be understood by all composites engineers. In the sections to follow, we will review the constitutive relations for isotropic materials in matrix form, then show that the extension to transversely isotropic composite laminae is very straightforward. Since each ply in a laminate may be oriented arbitrarily, we will then show how the elastic properties of the individual laminae can be transformed to a common direction. Finally, we will balance the individual ply stresses against the applied tractions and moments to develop matrix governing relations for the laminate as a whole. The calculations for laminate mechanics are best done by computer, and algorithms are outlined for elastic laminates, laminates exhibiting thermal expansion effects, and laminates exhibiting viscoelastic response. Isotropic linear elastic materials As shown in elementary texts on Mechanics of Materials (cf. Roylance ), the Cartesian strains resulting from a state of plane stress (σ = τ = τ =0)are 1 ɛ = (σ νσ ) 1 ɛ = (σ νσ ) 1 γ = τ In plane stress there is also a strain in the direction due to the Poisson effect: ɛ = ν (σ + σ ); this strain component will be ignored in the sections to follow. In the above relations there are three elastic constants: the Young's modulus, Poisson's ratio ν, and the shear modulus 1 See References listed at the end of this document. 1
2 . However, for isotropic materials there are only two independent elastic constants, and for instance can be obtained from and ν as = 2(1 + ν) Using matrix notation, these relations can be written as > < ɛ => 1 ν/ 0 σ ɛ = 6 > 7 < => ν/ 1 0 σ (1) :> > 4 5 γ ; >: τ >; The quantity in brackets is called the compliance matrix of the material, denoted S or. It is important to grasp the physical significance of its various terms. Directly from the rules of matrix multiplication, the element in the th row and th column of is the contribution of the th stress to the th strain. For instance the component in the 1,2 position is the contribution of the direction stress to the direction strain: multiplying σ by 1 gives the direction strain generated by σ, and then multiplying this by ν gives the Poisson strain induced in the direction. The zero elements show the lack of coupling between the normal and shearing components. If we wish to write the stresses in terms of the strains, Eqn. 1 can be inverted to give: > < σ > = 1 ν 0 ɛ >< > = 6 σ = ν 1 0 ɛ (2) > : > 1 ν τ ; 0 0 (1 ν)2 >: γ >; where here has been replaced by 2(1 + ν). This relation can be abbreviated further as: σ = Dɛ (3) where D = S 1 is the stiffness matrix. Note that the Young's modulus can be recovered by taking the reciprocal of the 1,1 element of the compliance matrix S, but that the 1,1 position of the stiffness matrix D contains Poisson effects and is not equal to. Anisotropic Materials If the material has a texture like wood or unidirectionallyreinforced fiber composites as shown in Fig. 1, the modulus 1 in the fiber direction will typically be larger than those in the transverse directions ( 2 and 3 ). When 1 6= 2 6= 3, the material is said to be orthotropic. It is common, however, for the properties in the plane transverse to the fiber direction to be isotropic to a good approximation ( 2 = 3 ); such a material is called transversely isotropic. The elastic constitutive laws must be modified to account for this anisotropy, and the following form is an extension of the usual equations of isotropic elasticity to transversely isotropic materials: > < ɛ1 = > ν > σ 1 ɛ 2 = 6 7 < >= 4 ν σ2 > : > γ ; :> 12 τ >; 12 The parameter ν 12 is the principal Poisson's ratio; it is the ratio of the strain induced in the 2direction by a strain applied in the 1direction. This parameter is not limited to values less than 0.5 as in isotropic materials. Conversely, ν 21 gives the strain induced in the 1direction by 2 (4)
3 .. Figure 1: An orthotropic material. a strain applied in the 2direction. Since the 2direction (transverse to the fibers) usually has much less stiffness than the 1direction, a given strain in the 1direction will usually develop a much larger strain in the 2direction than will the same strain in the 2direction induce a strain in the 1direction. Hence we will usually have ν 12 >ν 21. There are five constants in the above equation ( 1, 2, ν 12, ν 21 and 12 ). However, only four of them are independent; since the matrix is symmetric, we have ν 21 2 = ν The simple form of Eqn. 4, with zeroes in the terms representing coupling between normal and shearing components, is obtained only when the axes are aligned along the principal material directions; i.e. along and transverse to the fiber axes. If the axes are oriented along some other direction, all terms of the compliance matrix will be populated, and the symmetry of the material will not be evident. If for instance the fiber direction is offaxis from the loading direction, the material will develop shear strain as the fibers try to orient along the loading direction. There will therefore be a coupling between a normal stress and a shearing strain, which does not occur in an isotropic material. Transformation of Axes It is important to be able to transform the axes to and from the \laboratory" frame to a natural material frame in which the axes might be labeled 1 2 corresponding to the fiber and transverse directions as shown in Fig. 2. Figure 2: Rotation of axes. As shown in elementary textbooks, the transformation law for Cartesian Cauchy stress can 3
4 be written: σ 1 = σ cos 2 θ + σ sin 2 θ +2τ sin θ cos θ σ 2 = σ sin 2 θ + σ cos 2 θ 2τ sin θ cos θ (5) τ12 = 2 2 (σ σ )sinθ cos θ + τ (cos θ sin θ) Where θ is the angle from the axis to the 1 (fiber) axis. These relations can be written in matrix form as <> σ 1 > = 2 > σ 6 σ 2 = < >= σ (6) :> τ ;> >: τ ; > where =cosθand =sinθ. This can be abbreviated as σ 0 = Aσ (7) where A is the transformation matrix in brackets above. This expression could be applied to threedimensional as well as twodimensional stress states, although the particular form of A given in Eqn. 6 is valid in two dimensions only (plane stress), and for Cartesian coordinates. Using either mathematical or geometric arguments, it can be shown that the components of infinitesimal strain transform by almost thesamerelations: > < ɛ1 > = >< ɛ >= ɛ 2 = A ɛ (8) >: 1 >; >: 1 γ γ >; The factor of 1/2 on the shear components arises from the classical definition of shear strain, which is twice the tensorial shear strain. This introduces some awkwardness into the transformation relations, which can be reduced by introducing the Reuter's matrix, defined as [R] = or [R] = (9) We can now write: > < ɛ1 => >< ɛ 1 > = >< ɛ >= > < ɛ > = 1 ɛ 2 = R ɛ 2 = RA ɛ = RAR ɛ :> ;> : > 1 > ; > : 1 ; > > γ12 2γ : >; 12 2γ γ Or ɛ 0 = RAR 1 ɛ (10) The transformation law for compliance can now be developed from the transformation laws for strains and stresses. By successive transformations, the strain in an arbitrary  direction is related to strain in the 12 (principal material) directions, then to the stresses in the 12 directions, and finally to the stresses in the  directions. The final grouping of transformation matrices relating the  strains to the  stresses is then the transformed compliance matrix in the  direction: 2 4
5 > < ɛ >= < > ɛ > = < > ɛ ɛ 1 ɛ = R ɛ = RA 1 1 => <> = > 1 1 ɛ2 = RA R ɛ 2 >: > ; > : 1 >; > : 1 >; >: > γ 2γ 2γ 12 γ ; >< σ 1 => >< σ = RA 1 R 1 = > > < σ => S σ2 = RA 1 R 1 SA σ S σ >: τ >; >: 12 τ >; >: τ ;> where S is the transformed compliance matrix relative to stiffness matrix relative to  axes:  axes. The inverse of S is D, the 1 S = RA 1 R 1 SA D = S (11) Example 1 Consider a ply of Kevlarepoxy composite with a stiffnesses 1 = 82, 2 =4, 12 =28(allGPa)and ν 12 =025. oriented at 30 from the axis. The stiffness in the direction can be found as the reciprocal of the 1,1 element of the transformed compliance matrix S, as given by Eqn. 11. The following shows how this can be done with Maple symbolic mathematics software (edited for brevity): Read linear algebra package > with(linalg): Define compliance matrix > S:=matrix(3,3,[[1/E[1],nu[21]/E[2],0],[nu[12]/E[1],1/E[2],0],[0,0,1/G[12]]]); Numerical parameters for Kevlarepoxy > Digits:=4;unprotect(E);E[1]:=82e9;E[2]:=4e9;G[12]:=2.8e9;nu[12]:=.25; nu[21]:=nu[12]*e[2]/e[1]; Compliance matrix evaluated > S2:=map(eval,S); := Transformation matrix > A:=matrix(3,3,[[c^2,s^2,2*s*c],[s^2,c^2,2*s*c],[s*c,s*c,c^2s^2]]); Trigonometric relations and angle > s:=sin(theta);c:=cos(theta);theta:=30*pi/180; Transformation matrix evaluated > A2:=evalf(map(eval,A)); := Reuter's matrix > R:=matrix(3,3,[[1,0,0],[0,1,0],[0,0,2]]); Transformed compliance matrix > Sbar:=evalf(evalm( R &* inverse(a2) &* inverse(r) &* S2 &* A2 )); 5
6 := Stiffness in xdirection > 'E[x]'=1/Sbar[1,1]; = Note that the transformed compliance matrix is symmetric (to within numerical roundoff error), but that nonzero coupling values exist. A user not aware of the internal composition of the material would consider it completely anisotropic. Laminated composite plates One of the most common forms of fiberreinforced composite materials is the crossplied laminate, in which the fabricator \lays up" a sequence of unidirectionally reinforced \plies" as indicated in Fig. 3. Each ply is typically a thin (approximately 0.2 mm) sheet of collimated fibers impregnated with an uncured epoxy or other thermosetting polymer matrix material. The orientation of each ply is arbitrary, and the layup sequence is tailored to achieve the properties desired of the laminate. In this section we outline how such laminates are designed and analyzed. Figure 3: A 3ply symmetric laminate. \Classical Laminate Theory" is an extension of the theory for bending of homogeneous plates, but with an allowance for inplane tractions in addition to bending moments, and for the varying stiffness of each ply in the analysis. In general cases, the determination of the tractions and moments at a given location will require a solution of the general equations for equilibrium and displacement compatibility of plates. This theory is treated in a number of standard texts 2,and will not be discussed here. We begin by assuming a knowledge of the tractions N and moments M applied to a plate at a position, as shown in Fig. 4: > < >= < > >= N = M = (12) ;> ;> >: >: 2 cf. S. Timoshenko and S. WoinowskyKrieger, Theory of Plates and Shells, McGrawHill, New York,
7 .. Figure 4: Applied moments in plate bending. It will be convenient to normalize these tractions and moments by the width of the plate, so they have units of N/m and Nm/m, or simply N, respectively. Coordinates and are the directions in the plane of the plate, and is customarily taken as positive downward. The def eflection in the direction is termed, also taken as positive downward... Figure 5: Displacement of a point in a plate (from Powell, 1983). Analogously with the Euler assumption for beams, the Kirshchoff assumption for plate bending takes initially straight vertical lines to remain straight but rotate around the midplane ( = 0). As shown in Fig. 5, the horizontal displacements and in the and directions due to rotation can be taken to a reasonable approximation from the rotation angle and distance from midplane, and this rotational displacement is added to the midplane displacement ( 0 0 ): = 0 0 (13) = 0 0 (14) The strains are just the gradients of the displacements; using matrix notation these can be written 7
8 >< ɛ => >< >= >< 0 0 >= 0 ɛ = ɛ = = 0 0 = ɛ + κ (15) :> >; : > > + ; : > γ (0 + 0 ) 2 >; 0 where ɛ 0 is the midplane strain and κ is the vector of second derivatives of the displacement, called the curvature: > < κ > = >< 0 >= κ = κ = 0 >: κ ; > : > 2 >; 0 The component κ is a twisting curvature, stating how the direction midplane slope changes with (or equivalently how the direction slope changes with ). The stresses relative to the  axes are now determined from the strains, and this must take consideration that each ply will in general have a different stiffness, depending on its own properties and also its orientation with respect to the  axes. This is accounted for by computing the transformed stiffness matrix D as described in the previous section (Eqn. 11). Recall that the ply stiffnesses as given by Eqn. 4 are those along the fiber and transverse directions of that particular ply. The properties of each ply must be transformed to a common  axes, chosen arbitrarily for the entire laminate. The stresses at any vertical position are then: σ = Dɛ = Dɛ 0 + Dκ (16) where here D is the transformed stiffness of the ply at the position at which the stresses are being computed. Each of these ply stresses must add to balance the traction per unit width N: Z N = +2 2 Z k σ = X +1 σ (17) =1 k where σ is the stress in the th ply and is the distance from the laminate midplane to the bottom of the th ply. Using Eqn. 16 to write the stresses in terms of the midplane strains and curvatures: X (Z k+1 Z k+1 ) N = Dɛ 0 + Dκ (18) =1 k k The curvature κ and midplane strain ɛ 0 are constant throughout, and the transformed stiffness D does not change within a given ply. Removing these quantities from within the integrals: X ( Z k+1 Z ) k+1 N = Dɛ 0 + Dκ =1 k k After evaluating the integrals, this expression can be written in the compact form: where A is an \extensional stiffness matrix" defined as: (19) N = Aɛ 0 + Bκ (20) 8
9 X A = D(+1 ) (21) =1 and B is a \coupling stiffness matrix" defined as: 1 X B = D( ) (22) =1 The rationale for the names \extensional" and \coupling" is suggested by Eqn. 20. The A matrix gives the influ nfluence of an extensional midplane strain ɛ 0 on the inplane traction N, and the B matrix gives the contribution of a curvature κ to the traction. It may not be obvious why bending the plate will require an inplane traction, or conversely why pulling the plate in its plane will cause it to bend. But visualize the plate containing plies all of the same stiffness, except for some very lowmodulus plies somewhere above its midplane. When the plate is pulled, the more compliant plies above the midplane will tend to stretch more than the stiffer plies below the midplane. The top half of the laminate stretches more than the bottom half, so it takes on a concavedownward curvature. Similarly, the moment resultants per unit width must be balanced by the moments contributed by the internal stresses: M = Z + 2 σ=bɛ 0 +Dκ (23) 2 where D is a \bending stiffness matrix" defined as: 1 D = X D( ) (24) =1 The complete set of relations between applied forces and moments, and the resulting midplane strains and curvatures, can be summarized as a single matrix equation: ( ) " #( ) N A B ɛ 0 = M B D κ The ABBD matrix in brackets is the laminate stiffness matrix, and its inverse will be the laminate compliance matrix. The presence of nonzero elements in the coupling matrix B indicates that the application of an inplane traction will lead to a curvature or warping of the plate, or that an applied bending moment will also generate an extensional strain. These effects are usually undesirable. However, they can be avoided by making the laminate symmetric about the midplane, as examination of Eqn. 22 can reveal. (In some cases, this extensioncurvature coupling can be used as an interesting design feature. For instance, it is possible to design a composite propeller blade whose angle of attack changes automatically with its rotational speed: increased speed increases the inplane centripetal loading, which induces a twist into the blade.) The above relations provide a straightforward (although tedious, unless a computer is used) means of determining stresses and displacements in laminated composites subjected to inplane traction or bending loads: 9 (25)
10 1. For each material type in the stacking sequence, obtain by measurement or micromechanical estimation the four independent anisotropic parameters appearing in Eqn. 4: ( 1, 2, ν 12,and 12 ). 2. Using Eqn. 11, transform the compliance matrix for each ply from the ply's principal material directions to some convenient reference axes that will be used for the laminate as awhole. 3. Invert the transformed compliance matrix to obtain the transformed (relative to  axes) stiffness matrix D. 4. Add each ply's contribution to the A, B and D matrices as prescribed by Eqns. 21, 22 and Input the prescribed tractions N and bending moments M, and form the system equations given by Eqn Solve the resulting system for the unknown values of inplane strain ɛ 0 and curvature κ. 7. Use Eqn. 16 to determine the ply stresses for each ply in the laminate in terms of ɛ 0, κ and. These will be the stresses relative to the  axes. 8. Use Eqn. 6 to transform the  stresses back to the principal material axes (parallel and transverse to the fibers). 9. If desired, the individual ply stresses can be used in a suitable failure criterion to assess the likelihood of that ply failing. The TsaiHill criterion is popularly used for this purpose: ( ) 2 ( ) 2 ( ) σ1 σ 1 σ 2 σ2 τ = 1 (26) σ^1 σ^2 1 σ^2 τ^12 Here σ^1 and σ^2 are the ply tensile strengths parallel to and along the fiber direction, and ^τ 12 is the intralaminar ply strength. This criterion predicts failure whenever the lefthandside of the above equation equals or exceeds unity. Example 2 The laminate analysis outlined above has been implemented in a code named plate, and this example demonstrates the use of this code in determining the stiffness of a twoply 0/90 layup of graphite/epoxy composite. Here each of the two plies is given a thickness of 0.5, so the total laminate height will be unity. The laminate theory assumes a unit width, so the overall stiffness and compliance matrices will be based on a unit cross section. > plate assign properties for lamina type 1... enter modulus in fiber direction... (enter 1 to stop): 230e9 enter modulus in transverse direction: 6.6e9 enter principal Poisson ratio:.25 enter shear modulus: 4.8e9 enter ply thickness:.5 assign properties for lamina type
11 enter modulus in fiber direction... (enter 1 to stop): 1 define layup sequence, starting at bottom... (use negative material set number to stop) enter material set number for ply number 1: 1 enter ply angle: 0 enter material set number for ply number 2: 1 enter ply angle: 90 enter material set number for ply number 3: 1 laminate stiffness matrix: E E E D D D E E E D D D E E E D D D E E E D D D E E E D D D E E E D D D+09 laminate compliance matrix: E E E D D D E E E D D D E E E D D D E E E D D D E E E D D D E E E D D D08 Note that this unsymmetric laminate generates nonzero values in the coupling matrix B, as expected. The stiffness is equal in the and directions, as can be seen by examing the 1,1 and 2,2 elements of the laminate compliance matrix. The effective modulus is = = =392GPa. However, the laminate is not isotropic, as can be found by rerunning plate with the 0/90 layup oriented at a different angle from the axes. Temperature Effects There are a number of improvements one might consider for the plate code described above: it could be extended to include interlaminar shear stresses between plies, it could incorporate a database of commercially available prepreg and core materials, or the user interface could be made \friendlier" and graphicallyoriented. Many such features are available in commercial codes, or could be added by the user, and will not be discussed further here. However, thermal expansion effects are so important in application that a laminate code almost must have this feature to be usable, and the general approach will be outlined here. In general, an increase in temperature causes a thermal expansion given by the wellknown relation ɛ = α,whereɛ is the thermallyinduced strain and α is the coefficient of 11
12 linear thermal expansion. This thermal strain is obtained without needing to apply stress, so that when Hooke's law is used to compute the stress from the strain the thermal component is subtracted first: σ = (ɛ α ). The thermal expansion causes normal strain only, so shearing components of strain are unaffected. Equation 3 can thus be extended as σ = D (ɛ ɛ ) where the thermal strain vector in the 1 2 coordinate frame is 8 9 > < α 1 >= ɛ = α 2 :> 0 >; Here α 1 and α 2 are the anisotropic thermal expansion coefficients in the fiber and transverse directions. Transforming to common axes, this relation becomes: >< σ => > ɛ σ = 12 α 64 7 < > = ɛ 5 4 α 5 (27) >: > τ ; > : 33 α >; The subscripts on the elements refer to row and column positions within the stiffness matrix rather than coordinate directions; the overbar serves as a reminder that these elements refer to  axes. The thermal expansion vector on the righthand side (α = α,α,α ) is essentially a strain vector, and so can be obtained from (α 1,α 2 0) as in Eqn. 10: <> α >= > < α 1 >= α = α = RA 1 R 1 α 2 :> ;> :> 0 >; α Note that in the common  direction, thermal expansion induces both normal and shearing strains. The previous temperatureindependent development can now be repeated, modified only by carrying along the thermal expansion terms. As before, the strain vector for any position from the midplane is given in terms of the midplane strain ɛ 0 and curvature κ by The corresponding stress is then σ ɛ = ɛ 0 + κ = D(ɛ 0 + κ α ) Balancing the stresses against the applied tractions and moments as before: Z Z N = σ = Aɛ + Bκ Dα Z M= Z σ=bɛ +Dκ Dα This result is identical to that of Eqns. 20 and 23, other than the addition of the integrals representing the \thermal loads." This permits temperaturedependent problems to be handled by an \equivalent mechanical formulation;" the overall governing equations can be written as 12
13 ( ) " #( ) A B ɛ 0 = N M B D κ or ( ɛ 0 where the \equivalent thermal loads" are given as Z N = N + Dα Z M=M+ κ ) Dα = " A B # 1 ( B D N M ) (28) The extension of the plate code to accommodate thermal effects thus consists of modifying the 6 1 loading vector by adding the two 3 1 vector integrals in the above expression. Viscoelastic Effects Since the matrix of many composite laminates is polymeric, the designer may need to consider the possibility of viscoelastic stress relaxation or creep during loading. Any such effect will probably not be large, since the fibers that bear most of the load are not usually viscoelastic. Further, the matrix material is usually used well below its glass transition temperature, and will act in a glassy elastic mode. Some applications may not be so simple, however. If the laminate is used at elevated temperature, and if stresses act in directions not supported by the reinforcing fibers, relaxation effects may be observed. Figure 6 shows creep measured in a T300/5208 unidirectional graphiteepoxy laminate 3, loaded transversely to the fibers at 149 C. Even in this almostworst case scenario, the creep strains are relatively small (less than 10% of the elastic strain), but Fig. 6 does show that relaxation effects may be important in some situations. Figure 6: Creep/creeprecovery response of graphiteepoxy laminate. 3 M.E. Tuttle and H.F. Brinson, \Prediction of LongTerm Creep Compliance of General Composite Laminates," Experimental Mechanics, p. 89, March
14 The TuttleBrinson paper cited above describes a timestepping computational scheme that can be used to model these viscoelastic laminate effects, and a simplified form of their method will be outlined here. The viscoelastic creep strain occurring in a given ply during a time increment can be calculated from the stress in the ply at that time, assuming the ply to be free of adjoining plies; this gives an independentply creep strain. This strain will act to relax the ply stress. Of course, the plies are not free to strain arbitrarily, and the proper strain compatibility can be reestablished by calculating the external loads that would produce elastic strains equal to the independentply creep strains. These loads are summed over all plies in the laminate to give an equivalent laminate creep load. This load is applied to the laminate to compute a set of compatible strains and curvatures, termed the equivalentlaminate creep strain. This strain is added to the initial elastic strain in computing the stress on a given ply, while the independentply creep strain is subtracted. The following list develops these steps in more detail: 1. The elastic midplane strains and curvatures are solved for the specified bending moments and tractions, using the glassy moduli of the various plies. From Eqn. 25: ( ) " # 1 ɛ 0 A B = κ B D ( N M ) 2. The elastic strain in each ply is then obtained from Eqn. 15. For the ply, with center at coordinate, thisis: 0 ɛ = ɛ + κ where the subscript indicates ply, elastic, strain in the xy direction. The elastic ply strains relative to the 12 (fibertransverse) directions are given by the transformation of Eqn. 10: ɛ 12 = RAR 1 ɛ These first two steps are performed by the elastic plate code, and the adaptation to viscoelastic response consists of adding the following steps. 3. The current ply stress σ 12 in the 12 directions is: σ 12 = D [ɛ 12 +(ɛ 12 ɛ 12 )] The quantity ɛ 12 ɛ 12 is the difference between the equivalent laminate creep strain and the independentply creep strain. The quantities ɛ 12 and ɛ 12 are set to zero initially, but are updated in steps 4 and 8 below to account for viscoelastic relaxation. 4. The current ply stress in then used in an appropriate viscoelastic model to compute the creep that would occur if the ply were free to strain independently of the adjoining plies; this is termed the independent ply creep strain. For a simple Voigt model, the current value of creep strain can be updated from its value in the previous time step as: ( ) ɛ = σ 1 dt/τ 1 dt/τ + ɛ where the superscripts on strain indicate values at the current and previous time steps. Here is the viscoelastic creep compliance and τ is a relaxation time. A creep strain 14
15 equal to will develop in addition to the initial elastic strain in the laminate, and a fraction 2 of this creep strain will develop in a time τ. Different values of will be used for the fiber, transverse, and shear strain components due to the anisotropy of the ply. 5. The stresses in the 12 and xy directions that would be needed to develop the independentply creep strains if the ply were elastic are σ σ 12 = Dɛ 12 = A 1 σ These equivalent elastic ply stresses are summed over all plies in the laminate to build up an equivalent laminate creep load. The contribution of the ply is: N = N + σ M = M + σ where is the thickness of the ply and is its centerline coordinate. 7. An equivalent laminate creep strain is then computed from the elastic compliance matrix and the equivalent laminate creep loads as ( ) " # ɛ 0 1 ( ) A B N = κ B D M 8. The ply laminate creep strain in the xy and 12 directions are ɛ ɛ = ɛ 0 + κ 12 = RAR 1 ɛ 9. Finally, the time is incremented ( + ) and another time cycle is computed starting at step 3. Example 3 As an illustration of the above algorithm, consider a simple model laminate with one isotropic ply. The elastic constants are = 100 (arbitrary units) and ν =025, and a unit stress is applied in the direction. The initial direction strain is therefore ɛ 0 = σ =001. In this isotropic test case, the code calculates the shear modulus as = 2(1 + ν). The creep strain is governed by a parameter, which sets the Voigt creep compliance to 2 in the transverse direction, 12 for shear components, and zero in the fiber direction (assuming only elastic response along the fibers.) Figure 7 shows the creep strain history of this laminate for a relaxation time of τ = 1000 s. The code steps linearly in log time, in this case with four time steps per decade. The creep strain is the strain over 4 and beyond the initial elastic strain, which transitions from zero to ɛ0 =5 10 as time progresses through the relaxation time. 15
16 Figure 7: Creep strain history in model laminate. References 1. Ashton, J.E., J.C. Halpin and P.H. Petit, Primer on Composite Materials: Analysis,Technomic Press, Westport, CT, Jones, R.M., Mechanics of Composite Materials, McGrawHill, New York, Powell, P.C, Engineering with Polymers, Chapman and Hall, London, Roylance, D., Mechanics of Materials, Wiley & Sons, New York, Problems 1. Write out the  twodimensional compliance matrix S and stiffness matrix D (Eqn. 11) for a single ply of graphite/epoxy composite with its fibers aligned along the  axes. 2. Write out the  twodimensional compliance matrix S and stiffness matrix D (Eqn. 11) for a single ply of graphite/epoxy composite with its fibers aligned 30 from the axis. 3. Plot the effective Young's modulus, measured along the axis, of a single unidirectional ply of graphiteepoxy composite as a function of the angle between the ply fiber direction and the axis. 4. Using a programming language of your choice, write a laminate code similar to the plate code mentioned in the text, and verify it by computing the laminate stiffness and compliance matrices given in Ex A ( ) layup (the S superscript indicates the plies are repeated to give a symmetric laminate) is an example of what are called \quasiisotropic" laminates, having equal stiffnesses in the and directions, regardless of the laminate orientation. Verify that this is so for two laminate orientations, one having the 0 plies oriented along the axis and the other with the 0 plies oriented at 30 from the axis. 16
17 Mechanical Properties of Composite Materials The following table lists physical and mechanical property values for representative ply and core materials widely used in fiberreinforced composite laminates. Ply properties are taken from F.P.Gerstle, \Composites," Encyclopedia of Polymer Science and Engineering, Wiley, New York, 1991, which should be consulted for data from a wider range of materials. See also G. Lubin, Handbook of Composites, Van Nostrand, New York, Sglass/ epoxy Kevlar/ epoxy HM Graphite/ epoxy Pine Rohacell 51 rigid foam Elastic Properties: 1,GPa ,GPa ,GPa ν Tensile Strengths: σ 1,MPa σ 2,Mpa σ 12,MPa Compressive Strengths: σ 1,MPa σ 2,MPa Physical Properties: α 1,10 6 / C α 2,10 6 / C Volume fraction Thickness, mm Density, Mg/m
18 MIT OpenCourseWare Mechanics of Materials Fall 1999 For information about citing these materials or our Terms of Use, visit:
Bending of Simply Supported Isotropic and Composite Laminate Plates
Bending of Simply Supported Isotropic and Composite Laminate Plates Ernesto GutierrezMiravete 1 Isotropic Plates Consider simply a supported rectangular plate of isotropic material (length a, width b,
More informationComposites Design and Analysis. Stress Strain Relationship
Composites Design and Analysis Stress Strain Relationship Composite design and analysis Laminate Theory Manufacturing Methods Materials Composite Materials Design / Analysis Engineer Design Guidelines
More informationQUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationDESIGN OF LAMINATES FOR INPLANE LOADING
DESIGN OF LAMINATES FOR INPLANOADING G. VERCHERY ISMANS 44 avenue F.A. Bartholdi, 72000 Le Mans, France Georges.Verchery@m4x.org SUMMARY This work relates to the design of laminated structures primarily
More informationMechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA What programs are in PROMAL? Master Menu The master menu screen with five separate applications from
More informationLAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS
XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds
More informationModule 4: Behaviour of a LaminaeII. Learning Unit 1: M1. M4.1 Mechanics of Composites. M4.1.1 Introduction to Mechanics of Composites
Module 4: Behaviour of a LaminaeII Learning Unit 1: M1 M4.1 Mechanics of Composites M4.1.1 Introduction to Mechanics of Composites The relation between ply uniaxial strengths and constituent properties
More informationChapter 2  Macromechanical Analysis of a Lamina. Exercise Set. 2.1 The number of independent elastic constants in three dimensions are: 2.
Chapter  Macromechanical Analysis of a Lamina Exercise Set. The number of independent elastic constants in three dimensions are: Anisotropic Monoclinic 3 Orthotropic 9 Transversely Orthotropic 5 Isotropic.
More informationModule 7: Micromechanics Lecture 29: Background of Concentric Cylinder Assemblage Model. Introduction. The Lecture Contains
Introduction In this lecture we are going to introduce a new micromechanics model to determine the fibrous composite effective properties in terms of properties of its individual phases. In this model
More informationMECHANICS OF MATERIALS. EQUATIONS AND THEOREMS
1 MECHANICS OF MATERIALS. EQUATIONS AND THEOREMS Version 20110114 Stress tensor Definition of traction vector (1) Cauchy theorem (2) Equilibrium (3) Invariants (4) (5) (6) or, written in terms of principal
More informationFinite Element Analysis of Composite Laminate By Using ABDH Matrix(Stiffness Matrix)
Finite Element Analysis of Composite Laminate By Using ABDH Matrix(Stiffness Matrix) Nikhil J. Chaudhari 1 Post Graduate Student Department of Mechanical Engineering Veermata Jijabai Technological Institute
More information2. Mechanics of Materials: Strain. 3. Hookes's Law
Mechanics of Materials Course: WB3413, Dredging Processes 1 Fundamental Theory Required for Sand, Clay and Rock Cutting 1. Mechanics of Materials: Stress 1. Introduction 2. Plane Stress and Coordinate
More informationVALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 )
VALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 ) Graham D Sims and William R Broughton Composites Design Data and Methods, Centre for Materials
More informationCellular solid structures with unbounded thermal expansion. Roderic Lakes. Journal of Materials Science Letters, 15, (1996).
1 Cellular solid structures with unbounded thermal expansion Roderic Lakes Journal of Materials Science Letters, 15, 475477 (1996). Abstract Material microstructures are presented which can exhibit coefficients
More information6. Bending CHAPTER OBJECTIVES
CHAPTER OBJECTIVES Determine stress in members caused by bending Discuss how to establish shear and moment diagrams for a beam or shaft Determine largest shear and moment in a member, and specify where
More informationPassive Damping Characteristics of Carbon Epoxy Composite Plates
Journal of aterials Science and Engineering A 6 (12) (2016) 3542 doi: 10.17265/21616213/2016.12.005 D DAVID PUBLISHIG Passive Damping Characteristics of Carbon Epoxy Composite Plates Dileep Kumar K
More informationComposite Laminate Modeling
omposite Laminate Modeling White Paper for Femap and NX Nastran Users Venkata Bheemreddy, Ph.D., Senior Staff Mechanical Engineer Adrian Jensen, PE, Senior Staff Mechanical Engineer WHAT THIS WHITE PAPER
More informationME 582 Advanced Materials Science. Chapter 2 Macromechanical Analysis of a Lamina (Part 2)
ME 582 Advanced Materials Science Chapter 2 Macromechanical Analysis of a Lamina (Part 2) Laboratory for Composite Materials Research Department of Mechanical Engineering University of South Alabama, Mobile,
More informationPresented By: EAS 6939 Aerospace Structural Composites
A Beam Theory for Laminated Composites and Application to Torsion Problems Dr. BhavaniV. Sankar Presented By: Sameer Luthra EAS 6939 Aerospace Structural Composites 1 Introduction Composite beams have
More informationModule 5: Laminate Theory Lecture 19: Hygro thermal Laminate Theory. Introduction: The Lecture Contains: Laminate Theory with Thermal Effects
Module 5: Laminate Theory Lecture 19: Hygro thermal Laminate Theory Introduction: In this lecture we are going to develop the laminate theory with thermal and hygral effects. Then we will develop the
More informationMESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP Wanil Byun*, Seung Jo Kim*, Joris Wismans** *Seoul National University, Republic
More informationUsing MATLAB to Design and Analyse Composite Laminates
Engineering, 2010, 2, 904916 doi:10.4236/eng.2010.211114 Published Online November 2010 (http://www.scirp.org/journal/eng). Using MATLAB to Design and Analyse Composite Laminates Abstract Avinash Ramsaroop,
More informationChapter 3. Load and Stress Analysis
Chapter 3 Load and Stress Analysis 2 Shear Force and Bending Moments in Beams Internal shear force V & bending moment M must ensure equilibrium Fig. 3 2 Sign Conventions for Bending and Shear Fig. 3 3
More informationFracture Mechanics of Composites with Residual Thermal Stresses
J. A. Nairn Material Science & Engineering, University of Utah, Salt Lake City, Utah 84 Fracture Mechanics of Composites with Residual Thermal Stresses The problem of calculating the energy release rate
More informationThe Accuracy of Characteristic Length Method on Failure Load Prediction of Composite Pinned Joints
, June 30  July 2, 2010, London, U.K. The Accuracy of Characteristic Length Method on Failure Load Prediction of Composite Pinned Joints O. Aluko, and Q. Mazumder Abstract An analytical model was developed
More informationStacking sequences for Extensionally Isotropic, Fully Isotropic and QuasiHomogeneous Orthotropic Laminates.
49th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics, and Materials 710 April 2008, Schaumburg, IL AIAA 20081940 Stacking sequences for Extensionally Isotropic, Fully Isotropic and QuasiHomogeneous
More informationTuesday, February 11, Chapter 3. Load and Stress Analysis. Dr. Mohammad Suliman Abuhaiba, PE
1 Chapter 3 Load and Stress Analysis 2 Chapter Outline Equilibrium & FreeBody Diagrams Shear Force and Bending Moments in Beams Singularity Functions Stress Cartesian Stress Components Mohr s Circle for
More informationElements of Polymer Structure and Viscoelasticity. David M. Parks Mechanics and Materials II February 18, 2004
Elements of Polymer Structure and Viscoelasticity David M. Parks Mechanics and Materials II 2.002 February 18, 2004 Outline Elements of polymer structure Linear vs. branched; Vinyl polymers and substitutions
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 15 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional
More informationBasic Energy Principles in Stiffness Analysis
Basic Energy Principles in Stiffness Analysis StressStrain Relations The application of any theory requires knowledge of the physical properties of the material(s) comprising the structure. We are limiting
More informationSANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS
SANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS de Aguiar, José M., josemaguiar@gmail.com Faculdade de Tecnologia de São Paulo, FATECSP Centro Estadual de Educação Tecnológica Paula Souza. CEETEPS
More informationCONSTITUTIVE RELATIONS FOR LINEAR ELASTIC SOLIDS
Chapter 9 CONSTITUTIV RLATIONS FOR LINAR LASTIC SOLIDS Figure 9.1: Hooke memorial window, St. Helen s, Bishopsgate, City of London 211 212 CHAPTR 9. CONSTITUTIV RLATIONS FOR LINAR LASTIC SOLIDS 9.1 Mechanical
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 16 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional
More informationMATERIAL MECHANICS, SE2126 COMPUTER LAB 4 MICRO MECHANICS. E E v E E E E E v E E + + = m f f. f f
MATRIAL MCHANICS, S226 COMPUTR LAB 4 MICRO MCHANICS 2 2 2 f m f f m T m f m f f m v v + + = + PART A SPHRICAL PARTICL INCLUSION Consider a solid granular material, a so called particle composite, shown
More informationBeam Models. Wenbin Yu Utah State University, Logan, Utah April 13, 2012
Beam Models Wenbin Yu Utah State University, Logan, Utah 8434130 April 13, 01 1 Introduction If a structure has one of its dimensions much larger than the other two, such as slender wings, rotor blades,
More informationFinite element modelling of infinitely wide Angleply FRP. laminates
www.ijaser.com 2012 by the authors Licensee IJASER Under Creative Commons License 3.0 editorial@ijaser.com Research article ISSN 2277 9442 Finite element modelling of infinitely wide Angleply FRP laminates
More informationPLY WAVINESS ON INPLANE STIFFNESS OF COMPOSITE LAMINATES
PLY WAVINESS ON INPLANE STIFFNESS OF COMPOSITE LAMINATES Cimini Jr., Carlos A., and Tsai, Stephen W. 2 Department of Mechanical Engineering, Federal University of Minas Gerais Av. Antônio Carlos, 6627
More informationEFFECT OF ELLIPTIC OR CIRCULAR HOLES ON THE STRESS DISTRIBUTION IN PLATES
EFFECT OF ELLIPTIC OR CIRCULAR HOLES ON THE STRESS DISTRIBUTION IN PLATES OF WOOD OR PLYWOOD CONSIDERED AS ORTHOTROPIC MATERIALS Information Revied and Reaffirmed March 1956 No. 1510 EFFECT OF ELLIPTIC
More informationFIXED BEAMS IN BENDING
FIXED BEAMS IN BENDING INTRODUCTION Fixed or builtin beams are commonly used in building construction because they possess high rigidity in comparison to simply supported beams. When a simply supported
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationA *69>H>N6 #DJGC6A DG C<>C::G>C<,8>:C8:H /DA 'D 2:6G  (  ) +"' ( + "( (' (& +" % '('%"' +"2 ( !"', % )% .C>K:GH>IN D; AF69>HH>6,+
The primary objective is to determine whether the structural efficiency of plates can be improved with variable thickness The large displacement analysis of steel plate with variable thickness at direction
More informationDEVELOPMENT OF A CONTINUUM PLASTICITY MODEL FOR THE COMMERCIAL FINITE ELEMENT CODE ABAQUS
DEVELOPMENT OF A CONTINUUM PLASTICITY MODEL FOR THE COMMERCIAL FINITE ELEMENT CODE ABAQUS Mohsen Safaei, Wim De Waele Ghent University, Laboratory Soete, Belgium Abstract The present work relates to the
More information3. BEAMS: STRAIN, STRESS, DEFLECTIONS
3. BEAMS: STRAIN, STRESS, DEFLECTIONS The beam, or flexural member, is frequently encountered in structures and machines, and its elementary stress analysis constitutes one of the more interesting facets
More informationEFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING
Journal of MECHANICAL ENGINEERING Strojnícky časopis, VOL 67 (217), NO 1, 522 EFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING Arnab Choudhury 1,
More informationCOMPUTER AIDED DESIGN IN CASE OF THE LAMINATED COMPOSITE MATERIALS
6 th International Conference Computational Mechanics and Virtual Engineering COMEC 15 1516 October 15, Braşov, Romania COMPUER AIDED DESIGN IN CASE OF HE LAMINAED COMPOSIE MAERIALS Camelia Cerbu ransilvania
More informationMATERIAL ELASTIC ANISOTROPIC command
MATERIAL ELASTIC ANISOTROPIC command.. Synopsis The MATERIAL ELASTIC ANISOTROPIC command is used to specify the parameters associated with an anisotropic linear elastic material idealization. Syntax The
More informationUnderstand basic stressstrain response of engineering materials.
Module 3 Constitutive quations Learning Objectives Understand basic stressstrain response of engineering materials. Quantify the linear elastic stressstrain response in terms of tensorial quantities
More informationMECHANICAL CHARACTERISTICS OF CARBON FIBER YACHT MASTS
MECHANICAL CHARACTERISTICS OF CARBON FIBER YACHT MASTS This paper provides a preliminary stress analysis of a carbon reinforced layered cylinder such as would be found in a yacht mast. The cylinder is
More informationA Study on the Tube of Integral Propeller Shaft for the Rearwheel Drive Automobile Using Carbon Composite Fiber
A Study on the Tube of Integral Propeller Shaft for the Rearwheel Drive Automobile Using Carbon Composite Fiber Kibong Han Mechatronics Department, Jungwon University, 85 Munmuro, Goesangun, South Korea.
More informationTensile behaviour of antisymmetric CFRP composite
Available online at www.sciencedirect.com Procedia Engineering 1 (211) 1865 187 ICM11 Tensile behaviour of antisymmetric CFRP composite K. J. Wong a,b, *, X. J. Gong a, S. Aivazzadeh a, M. N. Tamin b
More informationEnhancing Prediction Accuracy In Sift Theory
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department
More informationDiscontinuous Distributions in Mechanics of Materials
Discontinuous Distributions in Mechanics of Materials J.E. Akin, Rice University 1. Introduction The study of the mechanics of materials continues to change slowly. The student needs to learn about software
More informationCalculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites
Copyright c 2007 ICCES ICCES, vol.1, no.2, pp.6167, 2007 Calculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites K. Gordnian 1, H. Hadavinia 1, G. Simpson 1 and A.
More information3D and Planar Constitutive Relations
3D and Planar Constitutive Relations A School on Mechanics of Fibre Reinforced Polymer Composites Knowledge Incubation for TEQIP Indian Institute of Technology Kanpur PM Mohite Department of Aerospace
More informationCHAPTER 6 BENDING Part 1
Ishik University / Sulaimani Civil Engineering Department Mechanics of Materials CE 211 CHAPTER 6 BENDING Part 11 CHAPTER 6 Bending Outlines of this chapter: 6.1. Chapter Objectives 6.2. Shear and
More informationOverview of Hygrothermally Stable Laminates with Improved Extensiontwist Coupling
Overview of Hygrothermally Stable Laminates with Improved Extensiontwist Coupling R. Haynes epartment of erospace Engineering, Georgia Institute of Technology 27 Ferst rive W, tlanta, G 33325, US robert.haynes@gatech.edu
More informationPRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses
OPTIMAT BLADES Page 1 of 24 PRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses first issue Peter Joosse CHANGE RECORD Issue/revision date pages Summary of changes draft 241002
More informationTesting and Analysis
Testing and Analysis Testing Elastomers for Hyperelastic Material Models in Finite Element Analysis 2.6 2.4 2.2 2.0 1.8 1.6 1.4 Biaxial Extension Simple Tension Figure 1, A Typical Final Data Set for Input
More informationInternational Journal of Advanced Engineering Technology EISSN
Research Article INTEGRATED FORCE METHOD FOR FIBER REINFORCED COMPOSITE PLATE BENDING PROBLEMS Doiphode G. S., Patodi S. C.* Address for Correspondence Assistant Professor, Applied Mechanics Department,
More informationCHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles
CHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles Mark Hughes 14 th March 2017 Today s learning outcomes To understand the role of reinforcement, matrix and
More informationLecture 7, Foams, 3.054
Lecture 7, Foams, 3.054 Opencell foams StressStrain curve: deformation and failure mechanisms Compression  3 regimes  linear elastic  bending  stress plateau  cell collapse by buckling yielding
More informationTHE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH
THE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH M. R. Wisnom University of Bristol Advanced Composites Centre for Innovation and Science University Walk, Bristol BS8 1TR, UK M.Wisnom@bristol.ac.uk
More informationPrediction of Delamination Growth Behavior in a Carbon Fiber Composite Laminate Subjected to Constant Amplitude CompressionCompression Fatigue Loads
Prediction of Delamination Growth Behavior in a Carbon Fiber Composite Laminate Subjected to Constant Amplitude CompressionCompression Fatigue Loads J. Raju 1*, D.S. Sreedhar 2, & C.M. Manjunatha 1 1
More informationFinite Element Analysis Prof. Dr. B. N. Rao Department of Civil Engineering Indian Institute of Technology, Madras. Module  01 Lecture  11
Finite Element Analysis Prof. Dr. B. N. Rao Department of Civil Engineering Indian Institute of Technology, Madras Module  01 Lecture  11 Last class, what we did is, we looked at a method called superposition
More information7.4 The Elementary Beam Theory
7.4 The Elementary Beam Theory In this section, problems involving long and slender beams are addressed. s with pressure vessels, the geometry of the beam, and the specific type of loading which will be
More informationCrash and Impact Simulation of Composite Structures by Using CAE Process Chain
Crash and Impact Simulation of Composite Structures by Using CAE Process Chain Madhukar Chatiri 1, Thorsten Schütz 2, Anton Matzenmiller 3, Ulrich Stelzmann 1 1 CADFEM GmbH, Grafing/Munich, Germany, mchatiri@cadfem.de
More informationCLASSICAL TORSION AND AIST TORSION THEORY
CLASSICAL TORSION AND AIST TORSION THEORY Background The design of a crane runway girder has not been an easy task for most structural engineers. Many difficult issues must be addressed if these members
More informationGeneric Strategies to Implement Material Grading in Finite Element Methods for Isotropic and Anisotropic Materials
University of Nebraska  Lincoln DigitalCommons@University of Nebraska  Lincoln Engineering Mechanics Dissertations & Theses Mechanical & Materials Engineering, Department of Winter 1292011 Generic
More informationKirchhoff Plates: Field Equations
20 Kirchhoff Plates: Field Equations AFEM Ch 20 Slide 1 Plate Structures A plate is a three dimensional bod characterized b Thinness: one of the plate dimensions, the thickness, is much smaller than the
More informationChapter 7. Highlights:
Chapter 7 Highlights: 1. Understand the basic concepts of engineering stress and strain, yield strength, tensile strength, Young's(elastic) modulus, ductility, toughness, resilience, true stress and true
More informationInfluence of the filament winding process variables on the mechanical behavior of a composite pressure vessel
Influence of the filament winding process variables on the mechanical behavior of a composite pressure vessel G. Vargas 1 & A. Miravete 2 1 Universidad Pontificia Bolivariana, Facultad de Ingeniería Mecánica,
More informationMECHANICS OF MATERIALS
Third E CHAPTER 2 Stress MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Texas Tech University and Strain Axial Loading Contents Stress & Strain:
More informationNonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. F Talence, France Le Cheylard, France
20 th International Conference on Composite Materials Copenhagen, 1924th July 2015 Nonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. Thierry Lorriot 1, Jalal El Yagoubi
More informationEsben Byskov. Elementary Continuum. Mechanics for Everyone. With Applications to Structural Mechanics. Springer
Esben Byskov Elementary Continuum Mechanics for Everyone With Applications to Structural Mechanics Springer Contents Preface v Contents ix Introduction What Is Continuum Mechanics? "I Need Continuum Mechanics
More informationMaterials: engineering, science, processing and design, 2nd edition Copyright (c)2010 Michael Ashby, Hugh Shercliff, David Cebon.
Modes of Loading (1) tension (a) (2) compression (b) (3) bending (c) (4) torsion (d) and combinations of them (e) Figure 4.2 1 Standard Solution to Elastic Problems Three common modes of loading: (a) tie
More information(MPa) compute (a) The traction vector acting on an internal material plane with normal n ( e1 e
EN10: Continuum Mechanics Homework : Kinetics Due 1:00 noon Friday February 4th School of Engineering Brown University 1. For the Cauchy stress tensor with components 100 5 50 0 00 (MPa) compute (a) The
More informationJeff Brown Hope College, Department of Engineering, 27 Graves Pl., Holland, Michigan, USA UNESCO EOLSS
MECHANICS OF MATERIALS Jeff Brown Hope College, Department of Engineering, 27 Graves Pl., Holland, Michigan, USA Keywords: Solid mechanics, stress, strain, yield strength Contents 1. Introduction 2. Stress
More informationEE C245 ME C218 Introduction to MEMS Design
EE C245 ME C218 Introduction to MEMS Design Fall 2007 Prof. Clark T.C. Nguyen Dept. of Electrical Engineering & Computer Sciences University of California at Berkeley Berkeley, CA 94720 Lecture 16: Energy
More informationPLAT DAN CANGKANG (TKS 4219)
PLAT DAN CANGKANG (TKS 4219) SESI I: PLATES Dr.Eng. Achfas Zacoeb Dept. of Civil Engineering Brawijaya University INTRODUCTION Plates are straight, plane, twodimensional structural components of which
More informationDESIGN OF COMPOSITE LAMINATED STRUCTURES BY POLAR METHOD AND TOPOLOGY OPTIMISATION
DESIGN OF COMPOSIE LAMINAED SUCUES BY POLA MEOD AND OPOLOGY OPIMISAION A. Jibawy,,3, C. Julien,,3, B. Desmorat,,4, (*), A. Vincenti UPMC Univ Paris 6, UM 79, Institut Jean Le ond d Alembert B.P. 6 4, place
More informationFlexuralTorsional Buckling of General ColdFormed Steel Columns with Unequal Unbraced Lengths
Proceedings of the Annual Stability Conference Structural Stability Research Council San Antonio, Texas, March 2124, 2017 FlexuralTorsional Buckling of General ColdFormed Steel Columns with Unequal
More informationContinuum Mechanics. Continuum Mechanics and Constitutive Equations
Continuum Mechanics Continuum Mechanics and Constitutive Equations Continuum mechanics pertains to the description of mechanical behavior of materials under the assumption that the material is a uniform
More informationSIMULATION OF PROGRESSIVE FAILURE PREDICTION OF FILAMENT WOUND COMPOSITE TUBES SUBJECTED TO MULTIPLE LOADING WITH MEMBRANEFLEXION COUPLING EFFECTS
VOL. 5, NO. 4, APRIL 010 ISSN 18196608 006010 Asian Research Publishing Network (ARPN). All rights reserved. SIMULATION OF PROGRESSIVE FAILURE PREDICTION OF FILAMENT WOUND COMPOSITE TUBES SUBJECTED TO
More informationMachine Direction Strength Theory of Corrugated Fiberboard
Thomas J. Urbanik 1 Machine Direction Strength Theory of Corrugated Fiberboard REFERENCE: Urbanik.T.J., Machine Direction Strength Theory of Corrugated Fiberboard, Journal of Composites Technology & Research,
More informationMATERIAL MECHANICS, SE2126 COMPUTER LAB 3 VISCOELASTICITY. k a. N t
MATERIAL MECHANICS, SE2126 COMPUTER LAB 3 VISCOELASTICITY N t i Gt () G0 1 i ( 1 e τ = α ) i= 1 k a k b τ PART A RELAXING PLASTIC PAPERCLIP Consider an ordinary paperclip made of plastic, as they more
More informationCurvature of a Cantilever Beam Subjected to an EquiBiaxial Bending Moment. P. Krulevitch G. C. Johnson
UCRLJC30440 PREPRINT Curvature of a Cantilever Beam Subjected to an EquiBiaxial Bending Moment P. Krulevitch G. C. Johnson This paper was prepared for submittal to the Materials Research Society Spring
More informationGyroscopic matrixes of the straight beams and the discs
Titre : Matrice gyroscopique des poutres droites et des di[...] Date : 29/05/2013 Page : 1/12 Gyroscopic matrixes of the straight beams and the discs Summarized: This document presents the formulation
More informationChapter 12. Static Equilibrium and Elasticity
Chapter 12 Static Equilibrium and Elasticity Static Equilibrium Equilibrium implies that the object moves with both constant velocity and constant angular velocity relative to an observer in an inertial
More informationChapter 3 LAMINATED MODEL DERIVATION
17 Chapter 3 LAMINATED MODEL DERIVATION 3.1 Fundamental Poisson Equation The simplest version of the frictionless laminated model was originally introduced in 1961 by Salamon, and more recently explored
More informationIntroduction to Continuous Systems. Continuous Systems. Strings, Torsional Rods and Beams.
Outline of Continuous Systems. Introduction to Continuous Systems. Continuous Systems. Strings, Torsional Rods and Beams. Vibrations of Flexible Strings. Torsional Vibration of Rods. BernoulliEuler Beams.
More informationTHREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT
THREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT Víctor Martínez 1, Alfredo Güemes 2, Norbert Blanco 1, Josep Costa 1 1 Escola Politècnica Superior. Universitat de Girona. Girona, Spain (17071) 2
More informationMECHANICS OF MATERIALS. Prepared by Engr. John Paul Timola
MECHANICS OF MATERIALS Prepared by Engr. John Paul Timola Mechanics of materials branch of mechanics that studies the internal effects of stress and strain in a solid body. stress is associated with the
More informationISSN: ISO 9001:2008 Certified International Journal of Engineering Science and Innovative Technology (IJESIT) Volume 2, Issue 4, July 2013
Delamination Studies in FibreReinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering
More informationUSING A HOMOGENIZATION PROCEDURE FOR PREDICTION OF MATERIAL PROPERTIES AND THE IMPACT RESPONSE OF UNIDIRECTIONAL COMPOSITE
Volume II: Fatigue, Fracture and Ceramic Matrix Composites USING A HOMOGENIZATION PROCEDURE FOR PREDICTION OF MATERIAL PROPERTIES AND THE IMPACT RESPONSE OF UNIDIRECTIONAL COMPOSITE A. D. Resnyansky and
More information**********************************************************************
Department of Civil and Environmental Engineering School of Mining and Petroleum Engineering 333 Markin/CNRL Natural Resources Engineering Facility www.engineering.ualberta.ca/civil Tel: 780.492.4235
More informationStiffness Matrices, Spring and Bar Elements
CHAPTER Stiffness Matrices, Spring and Bar Elements. INTRODUCTION The primary characteristics of a finite element are embodied in the element stiffness matrix. For a structural finite element, the stiffness
More informationBasic concepts to start Mechanics of Materials
Basic concepts to start Mechanics of Materials Georges Cailletaud Centre des Matériaux Ecole des Mines de Paris/CNRS Notations Notations (maths) (1/2) A vector v (element of a vectorial space) can be seen
More information3D Compression Molding
Autodesk Simulation Moldflow Insight 2014 3D Compression Molding Executive summary In this work, the simulation results from a program developed for the threedimensional analysis of compression molding
More information2D damping predictions of fiber composite plates: Layup effects
Available online at www.sciencedirect.com Composites Science and Technology 68 (2008) 727 733 COMPOSITES SCIENCE AND TECHNOLOGY www.elsevier.com/locate/compscitech 2D damping predictions of fiber composite
More informationEnergy release rate analysis for adhesive and laminate double cantilever beam specimens emphasizing the effect of residual stresses
International Journal of Adhesion & Adhesives 20 (1999) 59 70 International Journal of Adhesion & Adhesives Energy release rate analysis for adhesive and laminate double cantilever beam specimens emphasizing
More information